Research Article | Open Access
Ramona Gheonea, Carmen Mak, Eleonora Cornelia Crasmareanu, Vasile Simulescu, Nicoleta Plesu, Gheorghe Ilia, "Surface Modification of SnO2 with Phosphonic Acids", Journal of Chemistry, vol. 2017, Article ID 2105938, 7 pages, 2017. https://doi.org/10.1155/2017/2105938
Surface Modification of SnO2 with Phosphonic Acids
The aim of the present work was the study of phosphonic acids grafting on the surface of SnO2 at different molar ratios. In this paper we describe the functionalization of SnO2 surfaces with phosphonic acids RPO(OH)2. The surface modification process was achieved by using phenyl-phosphonic acid (PPA) and vinyl-phosphonic acid (VPA). The synthesized materials were investigated by using FT-IR, TGA (in air and in nitrogen), EDX, ESEM, and TEM methods. This synthetic approach has many advantages: films with optical quality and controlled thickness can be obtained using low temperatures and cheap raw materials, by using “green chemistry” synthetic routes. The hybrid materials have structures diversity and fascinating applications, attracting attention for a long time, due to their potential.
Metal or metal oxide nanoparticles have unique characteristics compared to larger scale materials. For applications, it is necessary to stabilize or to give a particular function to such nanoparticles. Surface grafting of nanoparticles is an important challenge in chemistry  and is of great interest for optical and electric applications, but especially for their use in medicine.
Synthesis of organic-inorganic hybrid materials leads to combining physical and chemical properties of organic and inorganic components. Hybrid organic-inorganic films are an ideal material for those applications in which transparency and homogeneity are of primary concern, such as in optics and photonics [2, 3]. The synthetic methods have a central role in the development of new materials . Recent development in the field of nanoscience and nanotechnology has set a focus on synthetic approaches to complex assemblies of nanoparticles with applications in optics, electromagnetism, bioimaging, and pharmaceutics [5, 6].
Titanium dioxide nanomaterials are known for their numerous and diverse applications, which range from common products, as sunscreens, to advanced devices, as photovoltaic cells, and include many environmental and biomedical applications (photocatalytic degradation of pollutants, water purification, biosensing, and drug delivery). The importance of these applications increased the interest for the fabrication and characterization of TiO2 nanomaterials in the last decades [7–10].
The addition of tin oxide or zirconium oxide typically serves to increase the refractive index of the photocurable hybrid material and to control the synthesis conditions: this is important for applications in optics [11, 12]. This synthetic approach has many advantages: films with optical quality and controlled thickness can be obtained using low temperatures and cheap raw materials. Nanoparticles of a broad variety of main group and transition metal oxides form exceptionally stable surface complexes with the ligands incorporating phosphate or phosphonate moiety .
Organic-inorganic hybrids appear as a creative alternative to obtain new materials with unusual features. These materials are considered innovative advanced materials and promising applications are expected in many fields: optics, electronics, mechanics, membranes, protective coatings, catalysis, sensors, biology, catalysis, elaboration of solid phases for chromatography, organic synthesis on solid phases, and the modification of the surface properties of solids [14–26].
The nanostructure, the degree of organization, and the properties that can be obtained for such materials depend evidently on the chemical nature of their components, but they also depend on the synergy of these components. The design of organically modified surfaces is a rapidly expanding field of research in materials science in which the central purpose is access to materials possessing tunable properties in diverse areas (derivatization of substrates with reactive end groups for further modification, protective layers, analytical or biological sensors, catalysis, biomedical devices, solar batteries, etc.). The most commonly applied approach to the stabilization of metal oxide nanoparticles dispersions is based on grafting of organic molecules on their surface [27, 28].
This modification can be performed using traditional polymer coatings or layer by layer deposition of ionic species , but the next-generation technologies increasingly involve grafting onto the surface using appropriate functional molecules, thus providing a better control of the density and orientation of the organic component at the surface.
Titania-based adsorbents can be surface modified for potential uses in various applications using organic monolayers carrying a wide range of organic functionalities . Surface modification allows TiO2 nanoparticles to be stabilized in both aqueous  and hydrocarbon [31, 32] media. They have also been converted into hybrid organic-inorganic materials with a lot of potential applications in several fields [33, 34].
The modification of metal oxides surfaces (SnO2, TiO2, or ZrO2) with phosphonic acids is currently attracting growing interest in different areas as self-assembled monolayers  and ceramic membranes . The balance between surface complexation (grafting) and surface phase transformation (metal phosphonate phases)  depends strongly on the experimental conditions. The use of aqueous solutions of phosphonic acids may result in the formation of phosphonate phases instead of the simple grafting, depending on the conditions [36, 37].
This paper is focused on the synthesis of hybrid materials by grafting of SnO2 surfaces with phenyl-phosphonic acid and vinyl-phosphonic acid.
2.1. Materials and Methods
SnO2 (Carlo Erba), phenyl-phosphonic acid (PPA)-C6H5P(O) (OH)2 (Fluka), vinyl-phosphonic acid (VPA), C2H5PO3 (Merk), and water were used as purchased.
There were carried out four syntheses (S1–S4). The first three syntheses were performed with phenyl-phosphonic acid at different molar ratios SnO2 : PPA (1 : 1, 2 : 1, and 3 : 1). In the case of S4, vinyl-phosphonic acid was used at molar ratio SnO2 : VPA 2 : 1.
In a Berzelius flask containing 50 ml water, tin oxide was dispersed. The amount of SnO2 used was 0.5 g for S1, 1 g for S2, and S4 and 1.5 g for S3, respectively. Then, 0.55 g phenyl-phosphonic acid for S1, S2, and S3 (resp., 0.4 g vinyl-phosphonic acid for S4) was dissolved in 50 ml water and was added dropwise to the mixture, over a period of time of 20–30 minutes. The reaction mixture was left under stirring for 32–35 hours.
The reaction mixture was filtered in vacuum, resulting for all compounds in a light grey precipitate, while the filtrate is very clear. The precipitate was left to dry for 2-3 days to dryness, resulting in synthesis of S1@PPA, S2@PPA, S3@PPA, and S4@VPA.
(i)Jasco FT-IR 4200 Spectrometer, KBr support, was used for recording the spectra.(ii)Thermal analysis TGA-DTG-DTA (thermogravimetry) was carried out by changing the temperature between 20°C and 900°C, by using an 851-LF 1100-Mettler Toledo apparatus in airflow. It has a sensitivity of 1 μg. The maximum amount of the sample, which could be measured, is 5 g.(iii)SEM and EDX characterizations were made using a Jeol JSM 6400 Scanning Microscope coupled with an X-ray microanalyzer EXL II System Link Analytical with a detector of 133 eV.
3. Results and Discussion
The modification of SnO2 surfaces with phosphonic acids is attracting growing interest because of the applications of such hybrid materials in different fields. This work describes the study of phosphonic acids grafting on the surface of SnO2 at different molar ratios.
The surface modification process was achieved using phenyl-phosphonic acid (PPA) and vinyl-phosphonic acid (VPA). The synthesized materials were investigated by using FT-IR, TGA (in air and in nitrogen), EDX, ESEM, and TEM methods.
In (Figure 1) characteristic FT-IR spectra for phenyl-acid phosphonic (S1) and vinyl-phosphonic acid (S4) of synthesized grafting of the SnO2, there are intense absorption show bands at = 1145.47–1239.12 cm−1. In each of these spectra, we can clearly see the presence of important bands overlapping in the 987.37–997.01 cm−1 region, corresponding to the different vibration modes of the phosphonic acid confirming the grafting of the molecules on the surface. Unfortunately, the absorption bands in this region are too poorly defined to clearly identify them and eventually determine the way the bifunctional molecules bind the surface. In the = 3735.4–3736.4 cm−1 region of the spectra, very weak C–H asymmetric and symmetric stretching vibrations bands are observed around 3064.30 cm−1. The bands in the regions of 987.37 cm−1–997.01 cm−1 and 1646.91–1647.88 cm−1 were attributed to stretching and vibrations of the –Sn–O–Sn– group and at 3853.08 cm−1 were attributed for Sn–O–P indicating the formation of the grafting of acid phosphonic the SnO2. The band ascribed to superficial Sn–O vibrations appeared at 625.78 cm−1. In addition, the FT-IR spectrum of the phosphonic acid grafted on SnO2 shows bands at = 997.01 cm−1, = 3736.4 cm−1. These values are indicative of weakly organized monolayer. These results confirm the presence of the grafting of phosphonic acids on the SnO2. From the values obtained, it results that the functionalization of tin oxide surface occurred with a higher yield with phenyl-phosphonic acid (S1–S3) relative to vinyl-phosphonic acid (S4).
In order to fully characterize the synthesized hybrid materials EDX analysis was also performed. Based on this analysis, the presence of all the elements could be confirmed for all the samples, including the presence of the phosphorus, which proves that the hybrid material containing SnO2 and the phosphonic acid was indeed obtained.
In addition to the previous described measurements, EDX analysis was also studied (Figures 2–5). Based on this, in the cases of phenyl-phosphonic acid and vinyl-phosphonic acids grafted on the tin oxide magnetic nanoparticles, the presence of phosphorus can be observed in all analyzed samples.
The presence of phosphorus was confirmed for all the obtained samples (Figures 2–5). Based on this analysis, the presence of the combined material can be confirmed by the presence of Sn, P, O, and C in the spectra.
From ESEM results (Figure 6(a), S1, Figure 6(b), S2, Figure 6(c), S3, and Figure 6(d), S4), we can observe no differences in morphology for all analyzed samples because the structures are very similar. The different radicals from their structures could not influence ESEM images at this resolutions.
The TEM images (Figure 7(a), S1, Figure 7(b), S2, Figure 7(c), S3, and Figure 7(d), S4) confirmed the findings from ESEM measurements, in the way that all the samples showed similar morphology. This is expected because the samples’ structures were not very different. Only the radicals (phenyl, vinyl) could not change the morphology significantly, according to TEM resolutions.
It is obvious that the TGA curves show small weight loss in the temperature range 25–800°C, lower than 5% weight (Table 1).
Because the weight loss up to the temperature of 130°C is under 0.5% wt, the physically adsorbed water or trapped solvent was missing or was totally removed, due to the prior drying step. Over 200°C in the all samples a monotonous decrease can be observed and mass loss curves indicate the decomposition of organic moiety and SnO2 crystalline structure modifications. Each sample presents different weight loss over 200°C, associated especially with the nature of organic acids attached on the SnO2 surface (Table 1). The second and more intense exothermic peak is related to the thermal decomposition of the organic matter, just as observed in the TGA curves. This peak is attributed to the combustion of the organic material yielding basically CO2, P2O5, and H2O. Almost no weight loss is observed above 600°C, suggesting the formation of crystalline SnO2 as a decomposition product. Tin oxides are stable between 500°C and 800°C.
In air, for sample S1 from 130°C to 435°C and 435°C to 550°C, there are two small exothermic peaks, which correspond to 2.10% and 1.99% relative weight losses. At about 435°C, the decomposition rate increases sharply.
For sample S2 from 130°C to 390°C and 390°C to 550°C, there are two small exothermic peaks in the air, which correspond to 0.96% and 2.06% relative weight losses. At about 460°C, the decomposition process takes place with the higher rate.
Sample S3, in air from 130°C to 365°C and 365°C to 550°C, shows two small exothermic peaks corresponding to 0.60% and 2.06% relative weight losses, respectively. At about 475°C, the decomposition process takes place with the maximum rate.
Two small exothermic peaks corresponding to 0.94% and 1.50% relative weight losses are observed for sample S4 in air from 130°C to 405°C and 405°C to 550°C, respectively. At about 475°C, the decomposition rate is maximum.
In nitrogen, the samples present two major weight losses, presented in Table 1. The first weight loss is associated with the release of moisture (90–130°C). The temperature range 130–550°C presents a weight loss mainly attributed to the release of the structural water resulting from the bonded hydroxyl groups and to the other process like degradation of P–C bonds.
TGA data showed a high thermal stability for all the obtained compounds. The mass losses were below 5%. According to Figures 8 and 9 and Table 1, due to the lowest mass loss, the most stable compound was obtained at molar ratio SnO2 : PPA 3 : 1. On the other hand, at the same molar ratio of 2 : 1, the thermal stability was higher for the materials obtained with VPA, than in the case when PPA was used.
The grafting of the surface of SnO2 under “green” conditions by using water as solvent was investigated by FT-IR, EDX, ESEM, TEM, and TGA (in air and in nitrogen). From FT-IR spectra, it results that the grafting of tin oxide surface occurred with a higher yield when phenyl-phosphonic acid (S1–S3) was used, in comparison with vinyl-phosphonic acid (S4).
From EDX determinations, the presence of phosphorus was confirmed for all the obtained samples, resulting in that the grafting process of SnO2 on phosphonic acids took place. Based on this analysis, the presence of the combined material can be confirmed by the presence of Sn, P, O, and C in the spectra.
The images obtained with TEM and ESEM revealed the morphology of the synthesized nanoparticles and materials. From the images obtained with ESEM, we can observe no differences in morphology for all analyzed samples, because the structures are very similar. As expected, TEM images confirmed the findings from ESEM measurements, in the way that all the samples showed similar morphology.
TGA data indicate for samples S1–S4 a high thermal stability. For all samples the mass losses are under 5% wt and a monotonous decrease over 200°C takes place and indicates the decomposition of organic moiety and SnO2 crystalline structure modifications.
The types of inorganic surfaces which can be modified using phosphonic acid chemistry are summarized in the present paper, as well as the related mechanisms involved when attaching phosphonate groups onto these surfaces. This paper finally goes on to outline the richness of applications, which can be developed from the resulting functional materials. Indeed, grafting by phosphonic compounds would allow the introduction of more organic groups on the surface of SnO2.
The authors declare that they have no competing interests.
The authors acknowledge the financial support of the ITN project 290248 part of the EU-ITN network Mag(net)icFun, FP7 Marie Curie Actions, and part of Research Program 2, Project 2.2, of Institute of Chemistry Timisoara of the Romanian Academy.
- M.-A. Neouze and U. Schubert, “Surface modification and functionalization of metal and metal oxide nanoparticles by organic ligands,” Monatshefte fur Chemie, vol. 139, no. 3, pp. 183–195, 2008.
- P. G. Mingalyov and G. V. Lisichkin, “Chemical modification of oxide surfaces with organophosphorus(V) acids and their esters,” Russian Chemical Reviews, vol. 75, no. 6, pp. 541–557, 2006.
- R. Houbertz, “Nanophotonic materials: photonic crystals, plasmonics and metamaterials,” Applied Surface Science, vol. 247, pp. 504–512, 2005.
- M. Cargnello, T. R. Gordon, and C. B. Murray, “Solution-phase synthesis of titanium dioxide nanoparticles and nanocrystals,” Chemical Reviews, vol. 114, no. 19, pp. 9319–9345, 2014.
- N. A. Kotov, “The collective behavior of nanoscale building blocks,” ACS Nano, vol. 3, no. 6, pp. 1307–1308, 2009.
- B. Scholl, H. Y. Liu, B. R. Long et al., “Single particle quantum dot imaging achieves ultrasensitive detection capabilities for Western immunoblot analysis,” ACS Nano, vol. 3, no. 6, pp. 1318–1328, 2009.
- P. Coppens, Y. Chen, and E. Trzop, “Crystallography and properties of polyoxotitanate nanoclusters,” Chemical Reviews, vol. 114, no. 19, pp. 9645–9661, 2014.
- Z. Zhang and J. T. Yates, “Band bending in semiconductors: chemical and physical consequences at surfaces and interfaces,” Chemical Reviews, vol. 112, no. 10, pp. 5520–5551, 2012.
- M. A. Henderson and I. Lyubinetsky, “Molecular-level insights into photocatalysis from scanning probe microscopy studies on TiO2(110),” Chemical Reviews, vol. 113, no. 6, pp. 4428–4455, 2013.
- C. L. Pang, R. Lindsay, and G. Thornton, “Structure of clean and adsorbate-covered single-crystal rutile TiO2 surfaces,” Chemical Reviews, vol. 113, no. 6, pp. 3887–3948, 2013.
- G. Brusatin, M. Guglielmi, P. Innocenzi et al., “Microstructural and optical properties of sol-gel silica-titania waveguides,” Journal of Non-Crystalline Solids, vol. 220, no. 2-3, pp. 202–209, 1997.
- P. Innocenzi, A. Martucci, M. Guglielmi et al., “Optical and surface properties of inorganic and hybrid organic-inorganic silica-titania sol-gel planar waveguides,” Journal of Non-Crystalline Solids, vol. 259, no. 1–3, pp. 182–190, 1999.
- R. Pazik, R. Andersson, L. Kepiński, J.-M. Nedelec, V. G. Kessler, and G. A. Seisenbaeva, “Surface functionalization of the metal oxide nanoparticles with biologically active molecules containing phosphonate moieties. Case study of BaTiO3,” Journal of Physical Chemistry C, vol. 115, no. 20, pp. 9850–9860, 2011.
- H. Schmidt, A. Kaiser, H. Patzelt, and H. Sholze, “Mechanical and physical properties of amorphous solids based on (CH3)2SiO-SiO2 gels,” Le Journal de Physique Colloques, vol. 43, pp. 275–278, 1982.
- C. Sanchez and F. Ribot, “Hybrid organic-inorganic materials: a land of multidisciplinarity,” New Journal of Chemistry, vol. 18, pp. 1007–1047, 1994.
- C. Sanchez, F. Ribot, and B. Lebeau, “Molecular design of hybrid organic-inorganic nanocomposites synthesized via sol-gel chemistry,” Journal of Materials Chemistry, vol. 9, no. 1, pp. 35–44, 1999.
- B. M. Novak, “Hybrid nanocomposite materials—between inorganic glasses and organic polymers,” Advanced Materials, vol. 5, no. 6, pp. 422–433, 1993.
- U. Schubert, N. Hüsing, and A. Lorenz, “Hybrid inorganic-organic materials by sol-gel processing of organofunctional metal alkoxides,” Chemistry of Materials, vol. 7, no. 11, pp. 2010–2027, 1995.
- D. A. Loy and K. J. Shea, “Bridged polysilsesquioxanes. Highly porous hybrid organic-inorganic materials,” Chemical Reviews, vol. 95, no. 5, pp. 1431–1442, 1995.
- Y. Chujo, “Organic-inorganic hybrid materials,” Current Opinion in Solid State and Materials Science, vol. 1, no. 6, pp. 806–811, 1996.
- A. Morikawa, Y. Iyoku, M.-A. Kakimoto, and Y. Imai, “Preparation of new polyimide-silica hybrid materials via the sol-gel process,” Journal of Materials Chemistry, vol. 2, no. 7, pp. 679–689, 1992.
- Y. Chujo and T. Saegusa, “Organic polymer hybrids with silica gel formed by means of the sol-gel method,” in Macromolecules: Synthesis, Order and Advanced Properties, vol. 100 of Advances in Polymer Science, pp. 11–29, Springer, Berlin, Germany, 1992.
- J. D. Mackenzie and E. P. Bescher, “Structures, properties and potential applications of ormosils,” Journal of Sol-Gel Science and Technology, vol. 13, no. 1, pp. 371–377, 1998.
- F. Ribot and C. Sanchez, “Organically functionalized metallic oxo-clusters: structurally well-defined nanobuilding blocks for the design of hybrid organic-inorganic materials,” Comments on Inorganic Chemistry, vol. 20, no. 4–6, pp. 327–371, 1999.
- E. F. Vansant, P. Van der, and K. C. Voort, “Characterization and chemical modification of silica surface,” in Studies in Surface Science and Catalysis, vol. 93, Elsevier, Amsterdam, The Netherlands, 1993.
- D. E. De Vos, I. F. J. Vankelecom, and P. A. Jacobs, Eds., Chiral Catalyst Immobilisation and Recycling, Wiley-VCH, New York, NY, USA, 2001.
- D. P. Puzzo, L. D. Bonifacio, J. Oreopoulos, C. M. Yip, I. Manners, and G. A. Ozin, “Color from colorless nanomaterials: bragg reflectors made of nanoparticles,” Journal of Materials Chemistry, vol. 19, no. 21, pp. 3500–3506, 2009.
- Q. L. M. De Chermont, C. Chanéac, J. Seguin et al., “Nanoprobes with near-infrared persistent luminescence for in vivo imaging,” Proceedings of the National Academy of Sciences of the United States of America, vol. 104, no. 22, pp. 9266–9271, 2007.
- F. Caruso, Colloids and Colloid Assemblies: Synthesis, Modification, Organization and Utilization of Colloid Particles, vol. 277, Wiley-VCH, Weinheim, Germany, 1997.
- G. A. Seisenbaeva, I. V. Melnyk, N. Hedin et al., “Molecular insight into the mode-of-action of phosphonate monolayers as active functions of hybrid metal oxide adsorbents. Case study in sequestration of rare earth elements,” RSC Advances, vol. 5, no. 31, pp. 24575–24585, 2015.
- T. Arita, K.-I. Moriya, T. Yoshimura, K. Minami, T. Naka, and T. Adschiri, “Dispersion of phosphonic acids surface-modified titania nanocrystals in various organic solvents,” Industrial & Engineering Chemistry Research, vol. 49, no. 20, pp. 9815–9821, 2010.
- B. Faure, G. Salazar-Alvarez, A. Ahniyaz et al., “Dispersion and surface functionalization of oxide nanoparticles for transparent photocatalytic and UV-protecting coatings and sunscreens,” Science and Technology of Advanced Materials, vol. 14, no. 2, Article ID 023001, 2013.
- F. Song, Y. Zhao, H. Ding et al., “Capture of carbon dioxide by amine-loaded as-synthesized TiO2 nanotubes,” Environmental Technology, vol. 34, no. 11, pp. 1405–1410, 2013.
- F. Song, Y. Zhao, Y. Cao, J. Ding, Y. Bu, and Q. Zhong, “Capture of carbon dioxide from flue gases by amine-functionalized TiO2 nanotubes,” Applied Surface Science, vol. 268, pp. 124–128, 2013.
- W. Gao, L. Dickinson, C. Grozinger, F. G. Morin, and L. Reven, “Self-assembled monolayers of alkylphosphonic acids on metal oxides,” Langmuir, vol. 12, no. 26, pp. 6429–6435, 1996.
- J. Caro, M. Noack, and P. Kolsch, “Microporous mesoporous-chemically modified ceramic membranes,” Microporous and Mesoporous Materials, vol. 22, no. 1–3, pp. 321–332, 1998.
- E. Laiti, P. Persson, and L. O. Ohman, “Balance between surface complexation and surface phase transformation at the alumina/water interface,” Langmuir, vol. 14, no. 4, pp. 825–831, 1998.
Copyright © 2017 Ramona Gheonea et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.